The effect of Merpol surfactant on the morphology and performance of PES/PVP membranes: antibiotic separation
- 342 Downloads
The present study used modified nanofiltration (NF) membranes to remove the emerging contaminant of amoxicillin (AMX) from synthetic wastewater. For this purpose, Merpol surfactant and polyvinylpyrrolidone were added to the casting solutions to prepare flat sheet asymmetric polyethersulfone (PES) NF membranes through phase inversion process. Then, the effect of adding Merpol surfactant at different concentrations on the morphology, hydrophilicity, and pure water flux (PWF) of the membranes, as well as the separation of AMX from aqueous solutions was investigated. The characteristics of the prepared membranes were studied by scanning electron microscopy (SEM), field emission scanning electron microscopy (FESEM), contact angle (CA) measurement and performance tests. The obtained results approved the improved hydrophilicity of the PES membranes after adding Merpol surfactant to the casting solution. The findings also revealed a gradual increase in the average size of the membrane pores in sub-layer and thinner top layer, proportional to the increase of surfactant content in the solution. The results also confirmed the increase of PWF under the influence of surfactant increase. As a result, for the membrane containing 8 wt% Merpol additive, the lowest CA (52.08°), the highest PWF (76.31 L/m2 h), and maximum AMX excretion (97%) were achieved.
KeywordsAntibiotic Hydrophilicity Merpol Nanofiltration Polyethersulfone membrane
Membrane separation technology has been widely applied in various industries because of its advantages, such as low energy consumption, no phase transition, and easy to scale up [1, 2]. This technology is a promising solution for removal of the emerging contaminants .
Nanofiltration (NF) membranes have a selectivity capability in the region between reverse osmosis (RO) and ultrafiltration (UF), which make it possible to separate monovalent and divalent salts, as well as organic solutes with molecular weights up to 1000 g/mol . The use of this relatively new technology has grown steadily in recent years [5, 6]. This is mainly due to low energy consumption and the high efficiency of this separation technology, which has led to its widespread use in various industries, such as water softening, drinking-water purification, dye and antibiotic purification, salt removal, and waste treatment . Nanofiltration is also increasingly used in new water treatment programs. In addition, to have highly biologically stable water, NF membranes offer a very good removal of the organic micropollutants. The reason is that the molecular weight cut-off (MWCO) values of NF membranes are often in the same range as that of endocrine-disrupting compounds (EDCs), pharmaceutically active compounds (PhACs) and personal care products (PPCPs) [8, 9].
Polymeric membranes, which occupy the vast majority of the market for water treatment, suffer significantly from fouling . Fouling on the membrane surfaces has been regarded as the most serious problem on membrane filtration technologies .
Polyethersulfone (PES), due to its high chemical, thermal, and mechanical stability, has widely been used to synthesis membranes for a variety of applications . The main limiting factor for using this chemical compound is its low hydrophilicity, which increases membrane fouling [13, 14].
One way to modify the performance of PES nanofiltration membranes is to increase their hydrophilicity. So far, the impact of the increased hydrophilicity of the membrane surfaces and pore walls on the reduction or suppression of membrane fouling has been confirmed by many scholars around the world in recent years . Adding hydrophilic polymer additives, such as polymeric surfactants, to PES membranes is a widely accepted way to improve hydrophilicity of the membranes. Surfactants are surface-active agents, constituting the most important category of detergents . For this purpose, various surfactants have yet been introduced, including but not limited to, Pluronic F127 , Tween 80 , Tween 20 , Tetronic 1307 , Triton X100, CTAB and SDS , Brij S100  and Brij58 [21, 22].
Antibiotics have become emerging contaminants of aquatic ecosystems in recent years. These pollutants, even in small quantities, are dangerous due to their high persistence in aquatic ecosystems. Studies have revealed the inefficiencies of conventional wastewater treatment methods in eliminating this pollutant, as evidence of presenting antibiotic contaminants in natural environments have been reported from almost every corner of the world [23, 24]. The presence of such compounds in natural environments has raised concerns about their toxicity to humans and animals, as well as the emergence of bacteria and genes resistant to antibiotics [25, 26]. Nowadays, membrane filtration based on NF and RO membranes can be considered one of the most promising techniques known to remove antibiotic compounds . There are numerous studies that have confirmed the effectiveness of this approach in eliminating antibiotic compounds, such as amoxicillin (AMX). As such, Zazouli et al.  used two commercial NF membranes, namely SR2 and SR3, to compare their performance in rejection of AMX. According to their findings, the SR3 NF membranes had a better performance than SR2 in the removal of AMX. They reported a removal rate of 95% for SR3 NF membranes and 64.9% for SR2 NF membranes. In another study by Shahtalebi et al. , the performance of commercial NF4040 membrane in AMX removal was estimated to be 97%. Their results showed that the AMX content of the feed stream is an influential factor in the rejection of AMX antibiotics so that the removal efficiency will be lower at higher concentrations.
There is no previously published article regarding the effects of the addition of Merpol surfactant as hydrophilic additive on the fundamental characteristics of the PES nanofiltration membranes to remove antibiotics, such as AMX. Thus, in this study, the effect of adding this surfactant into the PES casting solution on the morphology, hydrophilicity, and pure water flux (PWF) of the membranes as well as the rejection of AMX was investigated in detail.
Chemicals and methods
List of chemicals used in this research
Company of producer
Molecular weight (g/mol)
Polyethersulfone (PES, Ultrason E6020P)
Polyvinylpyrrolidone (PVP 40)
White to yellow solid
“MERPOL®HCS” (hydrophilic-lipophilic balance (HLB) = 15)
Dana Pharmaceutical Company
464 g/l (20 °C)
1000 g/l (25 °C)
Composition of PES casting solution
PES conc. (wt%)
PVP 40 conc. (wt%)
Merpol conc. (wt%)
A film applicator was used to caste the prepared homogenous solution on a glass substrate to a thickness of 300 µm. Then the cast film was moved into the non-solvent bath for immersion precipitation at 0 °C temperature, for 24 h to complete the phase separation, where exchange between the solvent (NMP) and non-solvent (water) was induced. This was done to ensure complete removal or evaporation of the residual solvent from the membranes. In the end, the membranes were dried up by filter papers for 24 h at room temperature.
Measurement of contact angle
Calculation of water-membrane contact angle (CA) is necessary for evaluating the hydrophilic feature of the membranes. In this research, this parameter was measured directly by the CA instrument of G10 KRUSS type, made in Germany. It should be mentioned that in all measuring steps, distilled water was used as probe liquid.
Scanning electron microscopy (SEM)
Cross-sections of the membrane were prepared for careful examination by the scanning electron microscope (SEM), of KYKY-EM 3200 type, made in China. Once the membrane specimens were frozen by liquid nitrogen, they were fractured and sputter-coated with gold. Finally, the specimens were examined by SEM at 25 kV.
Field emission scanning electron microscopy (FESEM)
The surface morphologies of the membranes were observed by field emission scanning electron microscopy (FESEM, Hitachi S4800, Japan). Before FESEM analysis, the membrane samples were dehydrated through graded ethanol series and dried in vacuum oven adequately.
Membrane performance measurement
Pure water flux (PWF)
To check the performance of the prepared membranes, a lab-scale cross-flow system was used. The system was mainly comprised of a reservoir, a pump, and a membrane module. The study was performed in batch mode at a trans-membrane pressure of 10 bars. To estimate PWF, permeate was collected constantly in a measuring cylinder over certain intervals. The details of the experimental set-up and calculation of PWF have been described elsewhere .
The filtration experiments were conducted to investigate capability of the prepared PES membranes in the rejection of AMX antibiotics. The dissolution of the AMX antibiotic in distilled water was the first step in this experiment.
For this purpose, the AMX was dissolved in distilled water and its concentration was kept constant at 20 ppm. The experiments were conducted under trans-membrane pressure of 10 bars. the feed, permeate, and retentate streams were sampled to check their AMX content by means of UV–Vis spectrophotometer (T60, China) at λmax 660 nm . Accordingly, the amount of AMX removal was calculated in percent.
Results and discussion
As Fig. 2 suggests, the top layer structure shows a completely different structure depending on the amount of the surfactant present in the casting solution. Changes in the contents of the Merpol surfactant caused morphological changes in the membrane structures so that by increasing the amount of surfactant from 0 to 8 wt%, the thick and dense upper layer of the membrane was converted into a low-dense thin layer. However, the further increase of surfactant from 8 to 10 wt% had inverse effects and thickened the surface layer. The mechanism of membrane formation has already been described in previous studies, such as Saljoughi and Mousavi  and Saljoughi et al. [33, 34, 35]. In general, the addition of hydrophilic additives, such as Merpol, to the casting solution has two main effects on membrane morphology, which are discussed below in brief.
As a hydrophilic additive with nonsolvent properties, Merpol causes an increase in the thermodynamic instability of the casting solution. Once the cast films are immersed into the coagulation bath, the film surface will be coated by a layer of amphiphilic Merpol molecules. The presence of these molecules will reduce surface tension and, consequently, water molecules will be diffused, easily [30, 32]. Low affinity between PES and water molecules causes the formation of nuclei of a polymer-poor phase on the surface, which ultimately causes the repulsion of PES chains at the presence of surfactant molecules. These nuclei are surface porous builders. As long as the concentration of the polymer in the boundaries rises significantly and until the moment of solidification, the process of solvent and nonsolvent diffusional exchange will continue. This suggests that the addition of Merpol leads to the formation of more nuclei, resulting in more porosity in the surface (Fig. 3). The instantaneous demixing in the coagulation bath and the formation of more porous membrane structure is a clear consequence of the above effects.
Another important effect of Merpol is the increase in viscosity of the cast film. This increase in viscosity, during the solidification process, reduces solvent (NMP) and nonsolvent (water) diffusional exchange rate and prevents instantaneous demixing. The delayed demixing process suppresses macrovides and creates denser structures. What ultimately determines the characteristics of the membrane’s final structure depends on the priority of instantaneous or delayed demixing processes which in turn as discussed earlier depends on the concentration of Merpol surfactant in the cast solution.
Two key factors involved in the formation of thick and low porosity membrane structures, which include increased viscosity and priority of delayed demixing over instantaneous. This condition, in the present study, was observed when the surfactant content was increased from 8 to 10 wt%.
Membrane contact angle (CA)
Effect of Merpol surfactant on the hydrophilicity of the prepared membranes
PES conc. (wt%)
PVP 40 conc. (wt%)
Merpol conc. (wt%)
Membrane performance in removal of AMX
All the membranes made with different amounts of Merpol surfactant have a better performance in antibiotic rejection than pure the membrane. As the surfactant is added to the casting solution, the membrane performance in the elimination of AMX antibiotic becomes better until it reaches its peak of 97% at 8 wt% Merpol content. Exceeding this amount, any further increase in the surfactant content does not lead to a positive effect on the AMX rejection performance; it even causes a performance loss. The mechanisms such as size exclusion, electrostatic charge repulsion, and adsorption, help to retain the organic solutes by NF membranes [4, 37]. The relatively hydrophilic nature of some pharmaceutical compounds such as antibiotics  prevents them from absorption by the surface of membranes.
As a result, the rejection of AMX can take place by steady-state rejection due to steric effects for uncharged solutes and integrated steric and electrostatic effects for charged solutes [21, 39]. In retention of pharmaceuticals by tight NF membranes, Stearic effects are dominant, while in loose NF membranes, both electrostatic repulsion and steric exclusion control the retention of ionizable pharmaceuticals .
There is a direct relationship between PWF and the number and size of pores in the membrane top layer . So, even the slightest change in the surface porosity will lead to much more fluctuations in the permeate flux . According to Fig. 5, the obtained results confirm the trends observed in the SEM images. As shown earlier in Fig. 2, the top layer thickness of the membranes after the addition of 2, 4, 6, and 8 wt% Merpol was decreased. This reduced the resistance of the membrane against water permeation and consequently, increased PWF. In membrane M6, containing 10 wt% Merpol, as a result of increasing the thickness of the upper layer, and thereby increasing the resistance to water penetration, the PWF is decreased.
Antibiotics have become emerging contaminants of aquatic ecosystems in recent years. These pollutants, even in small quantities, are dangerous due to their high persistence in aquatic ecosystems. Consequently, the removal of antibiotics before they enter the aquatic environment, as well as for water reuse is very pertinent.
This study investigated the morphology, wettability, PWF, and removal of AMX of the PES membranes after adding different concentrations of the Merpol surfactant. According to the research findings, adding Small amounts of the Merpol surfactant strongly improved the morphology and permeability of the PES membranes. Adding 2, 4, 6, and 8 wt% Merpol surfactant resulted in the formation of more porous membranes with a higher permeability. Conversely, adding higher amounts of surfactant by 10 wt % to the casting solution suppressed the microvoids and formed a denser structure with less permeability. Adding the Merpol surfactant to the casting solution also increased the wettability of the membranes. Rejection of AMX was highly related to the characteristics of the membranes, so that the initial increase in Merpol concentration up to 8 wt % resulted in the higher rejection of AMX.
The authors sincerely thank the officials at Islamic Azad University, Quchan Branch, for their financial support and the provision of laboratory equipment and space.
- 1.Yang X et al. (2018) Biomimetic silicification on membrane surface for highly efficient treatments of both oil-in-water emulsion and protein wastewater. Appl Mater Interfaces 10(35):29982–29991Google Scholar
- 2.Sun H et al (2018) Segregation-induced in situ hydrophilic modification of poly(vinylidene fluoride) ultrafiltration membranes via sticky poly(ethylene glycol) blending. J Membr Sci 563:22–30Google Scholar
- 3.Lan L et al (2019) High removal efficiency of antibiotic resistance genes in swine wastewater via nanofiltration and reverse osmosis processes. J Environ Manag 231:439–445Google Scholar
- 4.Ghaemi N et al (2012) Separation of nitrophenols using cellulose acetate nanofiltration membrane: influence of surfactant additives. Sep Purif Technol 85:147–156Google Scholar
- 5.Zhang W et al (2003) Development and characterization of composite nanofiltration membranes and their application in concentration of antibiotics. Sep Purif Technol 30(1):27–35Google Scholar
- 6.Bagheri H, Afkhami A, Noroozi A (2016) Removal of pharmaceutical compounds from hospital wastewaters using nanomaterials: a review. Anal Bioanal Chem Res 3(1):1–18Google Scholar
- 7.Yan C et al (2008) Preparation and characterization of chloromethylated/quaternized poly(phthalazinone ether sulfone ketone) for positively charged nanofiltration membranes. J Appl Polym Sci 107(3):1809–1816Google Scholar
- 8.Verliefde AR et al (2009) Influence of membrane fouling by (pretreated) surface water on rejection of pharmaceutically active compounds (PhACs) by nanofiltration membranes. J Membr Sci 330(1):90–103Google Scholar
- 9.Zazouli MA, Bazrafshan E (2015) Applications, issues and futures of nanofiltration for drinking water treatment. Health Scope 4(3):e27244Google Scholar
- 10.Low Z-X (2018) Fouling resistant 2D boron nitride nanosheet—PES nanofiltration membranes. J Membr Sci 563:949–956Google Scholar
- 11.Fatemeh Seyedpour S et al (2018) Low fouling ultrathin nanocomposite membranes for efficient removal of manganese. J Membr Sci 549:205–216Google Scholar
- 12.Rahman NA, Maruyama T, Matsuyama H (2008) Performance of polyethersulfone/tetronic-1307 hollow fiber membrane for drinking water production. J Appl Sci Environ Sanit 3:1–7Google Scholar
- 13.Rahimpour A, Madaeni SS (2010) Improvement of performance and surface properties of nano-porous polyethersulfone (PES) membrane using hydrophilic monomers as additives in the casting solution. J Membr Sci 360(1):371–379Google Scholar
- 14.Mahdavi H, Ardeshiri F (2016) An efficient nanofiltration membrane based on blending of polyethersulfone with modified (styrene/maleic anhydride) copolymer. J Iran Chem Soc 13(5):873–880Google Scholar
- 15.Amirilargani M, Saljoughi E, Mohammadi T (2010) Improvement of permeation performance of polyethersulfone (PES) ultrafiltration membranes via addition of Tween-20. J Appl Polym Sci 115(1):504–513Google Scholar
- 16.Ghaemi N et al (2012) Fabrication of cellulose acetate/sodium dodecyl sulfate nanofiltration membrane: characterization and performance in rejection of pesticides. Desalination 290:99–106Google Scholar
- 17.Peng J et al (2010) Effects of coagulation bath temperature on the separation performance and antifouling property of poly(ether sulfone) ultrafiltration membranes. Ind Eng Chem Res 49(10):4858–4864Google Scholar
- 18.Amirilargani M, Saljoughi E, Mohammadi T (2009) Effects of Tween 80 concentration as a surfactant additive on morphology and permeability of flat sheet polyethersulfone (PES) membranes. Desalination 249(2):837–842Google Scholar
- 19.Rahimpour A, Madaeni S, Mansourpanah Y (2007) The effect of anionic, non-ionic and cationic surfactants on morphology and performance of polyethersulfone ultrafiltration membranes for milk concentration. J Membr Sci 296(1):110–121Google Scholar
- 23.Homem V, Santos L (2011) Degradation and removal methods of antibiotics from aqueous matrices—a review. J Environ Manag 92(10):2304–2347Google Scholar
- 24.Egea-Corbacho A, Gutiérrez Ruiz S, Quiroga Alonso JM (2019) Removal of emerging contaminants from wastewater using nanofiltration for its subsequent reuse: full-scale pilot plant. J Clean Prod 214:514–523Google Scholar
- 26.Zazouli M et al (2010) Effect of hydrophilic and hydrophobic organic matter on amoxicillin and cephalexin residuals rejection from water by nanofiltration. Iran J Environ Health Sci Eng 7(1):15Google Scholar
- 27.Koyuncu I et al (2008) Removal of hormones and antibiotics by nanofiltration membranes. J Membr Sci 309(1):94–101Google Scholar
- 29.Shahtalebi A, Sarrafzadeh M, Rahmati MM (2011) Application of nanofiltration membrane in the separation of amoxicillin from pharmaceutical wastewater. Iran J Environ Health Sci Eng 8(2):109Google Scholar
- 30.Mousavi SM, Saljoughi E, Sheikhi-Kouhsar MR (2013) Preparation and characterization of nanoporous polysulfone membranes with high hydrophilic property using variation in CBT and addition of tetronic-1107 surfactant. J Appl Polym Sci 127(5):4177–4185Google Scholar
- 31.Al-Abachi MQ, Haddi H, Al-Abachi AM (2005) Spectrophotometric determination of amoxicillin by reaction with N,N-dimethyl-p-phenylenediamine and potassium hexacyanoferrate(III). Anal Chim Acta 554(1):184–189Google Scholar
- 32.Saljoughi E, Mousavi SM (2012) Preparation and characterization of novel polysulfone nanofiltration membranes for removal of cadmium from contaminated water. Sep Purif Technol 90:22–30Google Scholar
- 33.Saljoughi E, Amirilargani M, Mohammadi T (2010) Effect of PEG additive and coagulation bath temperature on the morphology, permeability and thermal/chemical stability of asymmetric CA membranes. Desalination 262(1):72–78Google Scholar
- 34.Saljoughi E, Amirilargani M, Mohammadi T (2009) Effect of poly(vinyl pyrrolidone) concentration and coagulation bath temperature on the morphology, permeability, and thermal stability of asymmetric cellulose acetate membranes. J Appl Polym Sci 111(5):2537–2544Google Scholar
- 35.Saljoughi E, Amirilargani M, Mohammadi T (2010) Asymmetric cellulose acetate dialysis membranes: synthesis, characterization, and performance. J Appl Polym Sci 116(4):2251–2259Google Scholar
- 36.Saljoughi E, Mohammadi T (2009) Cellulose acetate (CA)/polyvinylpyrrolidone (PVP) blend asymmetric membranes: preparation, morphology and performance. Desalination 249(2):850–854Google Scholar
- 37.Ghaemi N et al (2012) Effect of fatty acids on the structure and performance of cellulose acetate nanofiltration membranes in retention of nitroaromatic pesticides. Desalination 301:26–41Google Scholar
- 38.Urase T, Sato K (2007) The effect of deterioration of nanofiltration membrane on retention of pharmaceuticals. Desalination 202(1–3):385–391Google Scholar
- 39.Shah AD, Huang C-H, Kim J-H (2012) Mechanisms of antibiotic removal by nanofiltration membranes: model development and application. J Membr Sci 389:234–244Google Scholar
- 41.Mohammadi T, Saljoughi E (2009) Effect of production conditions on morphology and permeability of asymmetric cellulose acetate membranes. Desalination 243(1–3):1–7Google Scholar
- 42.Amirilargani M et al (2010) Effects of coagulation bath temperature and polyvinylpyrrolidone content on flat sheet asymmetric polyethersulfone membranes. Polym Eng Sci 50(5):885–893Google Scholar
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.